Elucidating the Phase Transformation of Li Lithiation at...
Embed Size (px)
Transcript of Elucidating the Phase Transformation of Li Lithiation at...
Elucidating the Phase Transformation of Li4Ti5O12 Lithiation at the Nanoscale Michael G. Verde,*,† Loïc Baggetto,‡,⊥ Nina Balke,§ Gabriel M. Veith,‡ Joon Kyo Seo,∥ Ziying Wang,†
and Ying Shirley Meng*,†
†Department of NanoEngineering, University of California San Diego, La Jolla, California 92093, United States ‡Materials Science and Technology Division, Oak Ridge National Laboratory, Oak Ridge, Tennessee 37831, United States §The Center for Nanophase Materials Sciences, Oak Ridge National Laboratory, Oak Ridge, Tennessee 37831, United States ∥Materials Science & Engineering Program, University of California San Diego, La Jolla, California 92093, United States
*S Supporting Information
ABSTRACT: This work provides insight regarding the fundamental lithiation and delithiation mechanism of the popular lithium ion battery anode material, Li4Ti5O12 (LTO). Our results quantify the extent of reaction between Li4Ti5O12 and Li7Ti5O12 at the nanoscale, during the first cycle. Lithium titanate’s discharge (lithiation) and charge (delithiation) reactions are notoriously difficult to characterize due to the zero-strain transition occurring between the end members Li4Ti5O12 and Li7Ti5O12. Interestingly, however, the latter compound is electronically conductive, while the former is an insulator. We take advantage of this critical property difference by using conductive atomic force microscopy (c-AFM) to locally monitor the phase transition between the two structures at various states of charge. To do so, we perform ex situ characterization on electrochemically cycled LTO thin-films that are never exposed to air. We provide direct confirmation of the manner in which the reaction occurs, which proceeds via percolation channels within single grains. We complement scanning probe analyses with an X-ray photoelectron spectroscopy (XPS) study that identifies and explains changes in the LTO surface structure and composition. In addition, we provide a computational analysis to describe the unique electronic differences between LTO and its lithiated form.
KEYWORDS: Li4Ti5O12, LTO, Li-ion battery, anode, thin-film, c-AFM, XPS
Due to the demand for high energy density batteries formobile electronics and electric vehicles, the quest forhigh capacity, low voltage anode materialsespecially involving Sihas been heavily pursued in recent years.1 In this respect, Li4Ti5O12 (lithium titanate, LTO) is viewed as an inferior lithium ion battery anode. It exhibits relatively low capacity and high voltage compared to the most commercially available Li-ion anode, graphite (175 vs 372 mAh·g−1 and 1.55 vs ∼0.1 V Li/Li+).2 Nevertheless, the same undesirable properties that contribute to low energy densities provide attractive advantages as well. Indeed, the high redox potential of LTO lies safely within the electrolyte stability window.3 This enables cycling without the formation of deleterious passivation
layers, which are a problem for the long-term stability of conventional graphite anode and the popular alternatives such as silicon.4 The two-phase reaction, which leads to moderate capacity, is also highly facile. It proceeds between two members (Li4Ti5O12 and Li7Ti5O12) that possess the same crystallo- graphic space group, Fd3 ̅m. Even upon intercalation of 3 Li+ per formula unit, there is only a 0.2% volume change of the spinel lattice, resulting in its description as a zero-strain material.5 The
Received: December 14, 2015 Accepted: March 15, 2016 Published: March 15, 2016
© 2016 American Chemical Society 4312 DOI: 10.1021/acsnano.5b07875 ACS Nano 2016, 10, 4312−4321
stability, robustness, and safety of LTO have in fact led to its successful commercialization.6
While the ionic conductivity of LTO is comparable to that of other Li-ion anodes, a major shortcoming is its inherently low electronic conductivity.7−10 Li4Ti5O12 is considered to be an insulator, with experimentally reported band gaps typically between 3.0 and 4.0 eV.11,12 To circumvent this problem, several strategies have been implemented. Coatings, such as carbon, have been applied to improve the electronic conductivity.13 Doping with a host of cations has also been performed to decrease the band gap and improve perform- ance.14−16 Alternatively, LTO nanostructures have been synthesized to shorten Li+ diffusion lengths and increase surface areas.17 The high surface area of nanoparticles typically promote two-phase reactions to proceed in order to minimize the large interface energy that would otherwise exist within small volume particles.18 When these treatments have been applied, extremely high reversible rates of up to 100C (full charge or discharge in almost 30 s) have been reported.19−21
Other work by Song et al. showed that even pristine LTO could be cycled fairly well without any form of modification.22 Kim et al. used an array of electrochemical and spectroscopic techniques to propose a mechanism responsible for this.23
Their hypotheses ultimately rest on the fact that LTO’s lithiated phase, Li7Ti5O12, is highly electronically conductive. If a small network of this phase forms upon initial discharge, it can enable an electronic pathway for further lithiation. Indeed, only a small extent of lithiation is required, as Young et al. have shown that at less than 5% capacity, LTO’s bulk electronic conductivity dramatically increases from about 10−7 to 10−1 S· cm−1.24
Understanding exactly how the phase transformation between Li4Ti5O12 and Li7Ti5O12 proceeds and what factors promote it is still relatively ill-defined. Because the lattice parameters of both structures are near identical, few diffraction techniques are able to physically differentiate them.25,26
Though rapid changes in bulk conductivity and light absorption have been observed upon minor lithiation, the exact mechanism that enables this is still not clear. The present study aims to exploit the most significant property difference between the two phases, their difference in electronic conductivity, in order to more fully explain the insulator−metal transition occurring within the system. Using conductive atomic force microscopy (c-AFM), we directly visualize the formation and distribution of each phase at the nanoscale, for the first time. We present comprehensive current and topography maps of LTO, at various states of charge, to demonstrate where the transition between these two phases occurs, and what features promote it. We also perform DFT calculations to more fully describe the reaction mechanism and structures formed. The band gaps of LTO and its lithiated form are calculated in order to confirm which phase is observed when conductivity is measured. These results are combined with chemistry-resolved surface measure- ments using X-ray photoelectron spectroscopy (XPS), at the same states of charge, to explain changes in surface morphology and composition. It is worth emphasizing that this study focuses on thin-film electrodes, which serve as a model system that possesses no binder or additive, in order to draw conclusions regarding the fundamental properties of LTO. The unique application of the scanning probe microscopy (SPM) methods presented here is a valuable key for the future
Figure 1. (A) Scanning electron microscopy (SEM) of a focused ion beam (FIB) cross section of the LTO thin-film and (B) top SEM image of the bare thin-film. Note that in (A) the top layer is a protective film used during FIB milling. (C) XRD pattern and Rietveld refinement of LTO thin film deposited onto Pt coated Al2O3 substrate. (D) Electrochemical profile of first cycle, with squares indicating points where samples were characterized, and first 10 cycles (inset).
ACS Nano Article
DOI: 10.1021/acsnano.5b07875 ACS Nano 2016, 10, 4312−4321
optimization of this material, its composite electrode, and others like it.
RESULTS AND DISCUSSION
Thin-Film Bulk Characteristics. The common use of conductive additives in LTO composite electrodes can strongly influence the manner in which its electrochemical reaction occurs. This is evidenced by the great deal of research dedicated to creating LTO−carbon composites.27−29 To determine how LTO’s fundamental mechanism proceeds, therefore, we made use of thin-films that possessed only the electrochemically active material. LTO was grown on Pt-coated (ca. 225 nm) Al2O3 disks using RF magnetron sputtering and exhibited a thickness around 800 nm (Figure 1A). The Pt layer was incorporated to ensure good electrical contact for use in batteries as well as for c-AFM analysis; furthermore, it does not oxidize during the high temperature preparation anneal. Figure 1B illustrates the particle size distribution of deposited LTO, which was 20−100 nm on average. The film was highly crystalline, as demonstrated by the grazing incidence X-ray diffraction (GIXRD) in Figure 1C. Some LTO peaks show uncharacteristically high intensities, such as the (400) and (511) indices, due to overlapping contributions from Al2O3 substrate. A three-phase fit, incorporating all materials, was performed in order to confirm their structures and lattice parameters (Figure 1C, Table S1). LTO, Pt, and Al2O3 were fit to space groups Fd3 ̅m, Fm3 ̅m, and R3̅c, respectively. The low residual, resulting in a conventional Rietveld factor (Rwp) of 7.18, confirms the purity of the film. The LTO lattice parameter was determined to be 8.3521 ± 0.0003, which is in excellent agreement with the values reported in literature.30
Figure 1D highlights the material’s first electrochemical cycle an